# Magnetic Materials (especially magnetic recording) Magnetic Materials (especially magnetic recording)

• View
6

0

Embed Size (px)

### Text of Magnetic Materials (especially magnetic recording) Magnetic Materials (especially magnetic...

• Magnetic Materials

(especially magnetic recording)

NSF Workshop on Introducing Science Faculty to Materials Science and Engineering

June 22, 2009

J.W.Harrell

Professor of Physics The University of Alabama

• Outline of talk

• What is magnetism?

• How can materials be magnetic?

• What are some important properties of magnetic materials?

• Magnetic recording – an important application of nanomagnetism

• Maxwell’s equation (SI units):

ρ = charge density J = current density ε = permittivity µ = permeability E = electric field (intrinsic field) D = displacement vector = εE (derived field) B = magnetic induction (intrinsic field) H = magnetic field = (1/µ)B (derived field)

• D = εE = ε0E + P, P = Σp/V = χE = polarization H = B/µ = B/µ0 – M, or B = µ0(H + M),

M = Σm/V = χmH = magnetization • SI units: B in tesla (T), H in A/m, M in A/m • Electromagnetic units (emu): a commonly used cgs

system that works best for magnetism (not the same as the Gaussian system)

emu system: B = H + 4πM, B in gauss (G), H in oersted (Oe), M in Oe (= emu/cm3)

Fields and Units

• Currents produce magnetic fields

Long, straight wire current loop (m = IA)

• F = qv x B dF = Idl x B

Magnetic fields exert forces on moving charges

• Interaction between a magnetic field and a magnetic dipole moment

A field exerts a torque on a magnetic dipole moment that tends to align the dipole in the field direction

B m

τ = m x B

A non-uniform field exerts a net force on a magnetic dipole moment.

F = -m(dB/dz)

• orbital: ml = -(e/2m)L

spin: ms = -(e/m)S

Bohr magneton:

Atomic origin of magnetism

• Permanent atomic moments in thermal equilibrium (Boltzmann distribution) in an external magnetic field – M = n, N = no. atoms per unit volume = average moment of atom U = -m.B = -mBcosθ = -mzB Classically,

Paramagnetism

(Quantum mechanics gives similar results.)

• Negative magnetic susceptibility exhibited by all substances. M = χH, (χ < 0)

Based on Faraday’s law: Electronic orbits change when magnetic field is applied to produce an opposing magnetic flux. Conduction electrons also exhibit diagmagnetism. χ is approximately independent of temperature.

Diagmagnetism

• Spontaneous magnetic ordering

Ferromagnetism: e.g., Co, Fe, Ni, NiFe, CoPt

Caused by exchange interactions between atoms

• Antiferromagnetism Ferrimagnetism

e.g., Fe3O4 (magnetite), γ-Fe2O3 (maghemite), BaFe12O19, TbFeCo

e.g., MnO, NiO, MnF2, α-Fe2O3 (hematite)

• • Magnetic ordering is due to exchange interaction between atoms. Exchange energy is the difference between the Coulomb interaction for antiparallel and parallel electrons

Eex = E↑↑ - E↑↓

Exchange interaction

• Net wavefunction (spin times spatial) of two electrons must be antisymmetrical (Pauli exclusion principle). Thus, spatial wavefunction for parallel and antiparallel spin configurations must have different symmetry – further apart when parallel.

Eex = -2JS1⋅S2,

J = exchange integral

• Where in the periodic table do we find magnetism?

• Slater-Pauling Curve

FeCo has highest known magnetization

(Ni)

(Co)(Fe)

(Mn)(Cr) (Cu)

• Some Important Properties of Ferro- and Ferri- Magnetic Materials

Intrinsic properties: •Saturation magnetization – Ms (A/m, emu/cc) •Magnetocrystalline anisotropy (J/m3, erg/cc) •Magnetostriction (unitless)

Extrinsic properties: •Coercivity (A/m, T, Oe) •Shape anisotropy (J/m3, erg/cc)

• Soft Magnetic Materials (low Hc)

• Important properties: Ms (usually want high), anisotropy (usually low), magnetostriction (usually small), frequency response (high), eddy current loss (low resistivity), …

• Examples: Iron and steel, NiFe, CoFe, amorphous alloys, ferrites, …

• Coercivity depends on both intrinsic properties and microstructure.

• Hard Magnetic Materials (high Hc)

• Applications: permanent magnets, magnetic recording media

• Examples: BaFe12O19, Fe14Nd2B, Sm2Co17, CoPtCr, … • Energy product = (BH)max • Coercivity depends on anisotropy and microstructure

• Magnetic domains

Large particles and films generally consist of uniformly magnetized regions (≥ 0.1 µm) called ‘domains’.

If particles are sufficiently small, then they are ‘single domain’. Critical size depends on strength of exchange coupling, magnetic anisotropy energy, magnetization, particle shape. DC ~ 10–100 nm.

Domain walls can move under the influence of an applied magnetic field.

• Hard Disk Drive

Magnetic film on which bits are stored.

Servo system for positioning the head

• Magnetic domains oriented in the direction of travel of the head.

Longitudinal Recording

Perpendicular Recording

Soft underlayer “mirrors” write head and makes it possible to write domains much closer together.

• 2004

2002

2006 2008

2010 2012: 4.4 nm x 4.4 nm

50 nm

400 nm

The incredible shrinking bit! Predicted Relative Sizes of HDD Storage Bits

(assumes areal densities continue to double yearly – but this is no longer occuring)

• Typical media layer structure

• lubricant

• diamond-like protection from wear and corrosion

• Co-alloy (CoPtCr, CoPtCrB, CoPtCrTa, …)

• Usually CrX. Helps improve epitaxial growth of magnetic layer, improves grain isolation by Cr diffusion from intermediate layer

• grain growth and texture (e.g., CrTi, CrTiB, NiAl)

• helps control grain growth and texture (CrX, e.g., CoCrZr)

• glass or NiP coated Al-Mg. Condition of NiP coating (oxidation, roughness) has some effect on grain size.

• Magnetic Media Evolution

0

0.2500

0 35

no rm

al iz

ed fr

eq ue

nc y

grain size (nm)

24 Gbit/in2 10 nm mean

16 Gbit/in2 11 nm mean

10 Gbit/in2 12 nm mean

6 Gbit/in2 15 nm mean

100 Gbit/ in2 9.1 nm mean

45 Gbit/ in2 9 nm mean

Physical grain size below 10 nm

• Ideal Media Structure

• For high-density storage, media should have small, isolated, thermally stable magnetic grains.

• Small grain size ⇒ magnetization decay; large write versus store fields ⇒ magnetic anisotropy must be increased.

• The problem with small magnets -

• Magnets no longer stay magnetized when they approach the nanometer size (superparamagnetism)

• Hard drive disks now made of cobalt alloy granular films. Small size limit is about 8 nanometers.

• One proposed solution for extending storage densities – Chemically synthesized FePt nanoparticles.

• Most materials have a preferred direction of magnetization. Usually, due to crystalline structure (cubic, hexagonal, etc.), shape (grains, films, etc.), or stress. Anisotropy energy = energy difference between “easy” and “hard” directions.

Magnetic anisotropy

• Self-organized FePt nanoparticles

• First reported by Sun et al. [Science, 287, 1989 (2000)] – one of “Chemistry Highlights” of 2000.

• Synthesis – reduction of Pt(acac)2 in a diol and decomposition of Fe (CO)5 in presence of surfactant stabilizers at high temperature.

• Self-assembly – slow evaporation of particle dispersion on substrate. 3.5 nm FePt particle array –

M. Chen and D.E. Nikles

10 nm

• High Anisotropy FePt Nanoparticle Arrays

• As prepared particles are superparamagnetic.

• Anneal at T ~ 550 oC to produce chemically ordered high- anisotropy L10 fct phase.

• Particles ≥ 3 nm thermally stable for > 10 years.

• Potential storage density > 1 Tb/in2 as conventional medium using heat assisted recording.

• Potential storage density ~ 50 Tb/in2 if 1 bit/particle recording can be achieved.

• Sintering of particles at the high annealing temperatures required for chemical ordering is a major problem.

• Library of Congress, Jefferson building

• the entire printed collection of the U.S. Library of Congress

50 terabits per square inch on a half dollar size disk

• Over 3.4 million high-resolution photos, or …

• 2,800 audio CDs, or…

• 1,600 hours of television, or …

http://en.wikipedia.org/wiki/Image:LOC_-_Jefferson_building.jpg http://en.wikipedia.org/wiki/Image:LOC_-_Jefferson_building.jpg

• Synthesis of FePt Nanoparticles

Courtesy of Hao Zeng (IBM)

Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents